LMucko/crystallography-open-database huggingface dataset:
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2373 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006740
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2373 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Ca O'
_chemical_name_mineral           Lime
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.969
_cell_length_b                   4.969
_cell_length_c                   4.969
_cell_formula_units_Z            4
_cell_volume                     122.689
_database_code_amcsd             0008322
_diffrn_ambient_temperature      2373
_exptl_crystal_density_diffrn    3.036
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006740
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2473 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006741
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2473 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Ca O'
_chemical_name_mineral           Lime
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.976
_cell_length_b                   4.976
_cell_length_c                   4.976
_cell_formula_units_Z            4
_cell_volume                     123.209
_database_code_amcsd             0008323
_diffrn_ambient_temperature      2473
_exptl_crystal_density_diffrn    3.023
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006741
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2573 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006742
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2573 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Ca O'
_chemical_name_mineral           Lime
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.987
_cell_length_b                   4.987
_cell_length_c                   4.987
_cell_formula_units_Z            4
_cell_volume                     124.028
_database_code_amcsd             0008324
_diffrn_ambient_temperature      2573
_exptl_crystal_density_diffrn    3.003
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006742
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2673 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006743
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2673 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Ca O'
_chemical_name_mineral           Lime
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.997
_cell_length_b                   4.997
_cell_length_c                   4.997
_cell_formula_units_Z            4
_cell_volume                     124.775
_database_code_amcsd             0008325
_diffrn_ambient_temperature      2673
_exptl_crystal_density_diffrn    2.985
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006743
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2773 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006744
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2773 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Ca O'
_chemical_name_mineral           Lime
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.009
_cell_length_b                   5.009
_cell_length_c                   5.009
_cell_formula_units_Z            4
_cell_volume                     125.676
_database_code_amcsd             0008326
_diffrn_ambient_temperature      2773
_exptl_crystal_density_diffrn    2.964
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006744
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 2973 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006745
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 2973 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Ca O'
_chemical_name_mineral           Lime
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.025
_cell_length_b                   5.025
_cell_length_c                   5.025
_cell_formula_units_Z            4
_cell_volume                     126.884
_database_code_amcsd             0008327
_diffrn_ambient_temperature      2973
_exptl_crystal_density_diffrn    2.936
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006745
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: Re wire, T = 3073 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006746
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: Re wire, T = 3073 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Ca O'
_chemical_name_mineral           Lime
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.030
_cell_length_b                   5.030
_cell_length_c                   5.030
_cell_formula_units_Z            4
_cell_volume                     127.264
_database_code_amcsd             0008328
_diffrn_ambient_temperature      3073
_exptl_crystal_density_diffrn    2.927
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006746
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: IR wire, T = 298 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006747
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: IR wire, T = 298 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.210
_cell_length_b                   4.210
_cell_length_c                   4.210
_cell_formula_units_Z            4
_cell_volume                     74.618
_database_code_amcsd             0008329
_diffrn_ambient_temperature      298
_exptl_crystal_density_diffrn    3.588
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006747
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: IR wire, T = 421 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006748
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: IR wire, T = 421 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.216
_cell_length_b                   4.216
_cell_length_c                   4.216
_cell_formula_units_Z            4
_cell_volume                     74.938
_database_code_amcsd             0008330
_diffrn_ambient_temperature      421
_exptl_crystal_density_diffrn    3.572
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006748
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: IR wire, T = 505 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006749
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: IR wire, T = 505 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.222
_cell_length_b                   4.222
_cell_length_c                   4.222
_cell_formula_units_Z            4
_cell_volume                     75.258
_database_code_amcsd             0008331
_diffrn_ambient_temperature      505
_exptl_crystal_density_diffrn    3.557
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006749
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: IR wire, T = 591 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006750
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: IR wire, T = 591 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.226
_cell_length_b                   4.226
_cell_length_c                   4.226
_cell_formula_units_Z            4
_cell_volume                     75.472
_database_code_amcsd             0008332
_diffrn_ambient_temperature      591
_exptl_crystal_density_diffrn    3.547
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006750
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: IR wire, T = 694 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006751
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: IR wire, T = 694 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.232
_cell_length_b                   4.232
_cell_length_c                   4.232
_cell_formula_units_Z            4
_cell_volume                     75.794
_database_code_amcsd             0008333
_diffrn_ambient_temperature      694
_exptl_crystal_density_diffrn    3.532
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006751
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: IR wire, T = 790 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006752
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: IR wire, T = 790 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.237
_cell_length_b                   4.237
_cell_length_c                   4.237
_cell_formula_units_Z            4
_cell_volume                     76.063
_database_code_amcsd             0008334
_diffrn_ambient_temperature      790
_exptl_crystal_density_diffrn    3.520
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006752
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: IR wire, T = 874 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006753
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: IR wire, T = 874 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.244
_cell_length_b                   4.244
_cell_length_c                   4.244
_cell_formula_units_Z            4
_cell_volume                     76.441
_database_code_amcsd             0008335
_diffrn_ambient_temperature      874
_exptl_crystal_density_diffrn    3.502
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006753
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: IR wire, T = 964 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006754
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: IR wire, T = 964 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.249
_cell_length_b                   4.249
_cell_length_c                   4.249
_cell_formula_units_Z            4
_cell_volume                     76.711
_database_code_amcsd             0008336
_diffrn_ambient_temperature      964
_exptl_crystal_density_diffrn    3.490
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006754
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: IR wire, T = 1052 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006755
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: IR wire, T = 1052 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.257
_cell_length_b                   4.257
_cell_length_c                   4.257
_cell_formula_units_Z            4
_cell_volume                     77.146
_database_code_amcsd             0008337
_diffrn_ambient_temperature      1052
_exptl_crystal_density_diffrn    3.470
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006755
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: IR wire, T = 1120 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006756
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: IR wire, T = 1120 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.261
_cell_length_b                   4.261
_cell_length_c                   4.261
_cell_formula_units_Z            4
_cell_volume                     77.363
_database_code_amcsd             0008338
_diffrn_ambient_temperature      1120
_exptl_crystal_density_diffrn    3.460
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006756
High-temperature thermal expansion of lime, periclase, corundum and spinel Sample: IR wire, T = 1211 K
Fiquet, G.; Richet, P.; Montagnac, G.; Physics and Chemistry of Minerals 27 (1999) 103–111; doi:10.1007/s002690050246

data_9006757
_publ_section_title
;
 High-temperature thermal expansion of lime, periclase,
 corundum and spinel
 Sample: IR wire, T = 1211 K
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              103
_journal_page_last               111
_journal_paper_doi               10.1007/s002690050246
_journal_volume                  27
_journal_year                    1999
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.267
_cell_length_b                   4.267
_cell_length_c                   4.267
_cell_formula_units_Z            4
_cell_volume                     77.691
_database_code_amcsd             0008339
_diffrn_ambient_temperature      1211
_exptl_crystal_density_diffrn    3.446
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9006757